#------------------------------------------------------------------------------
#$Date: 2025-08-21 03:19:08 +0300 (Thu, 21 Aug 2025) $
#$Revision: 301842 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/50/51/4505139.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4505139
loop_
_publ_author_name
'Upreti, Shailesh'
'Ramanan, Arunachalam'
_publ_section_title
;
 Structure-Directing Role of Hydrogen-Bonded Dimers of Phenylenediammonium
 Cations:  Supramolecular Assemblies of Octamolybdate-Based
 Organic−Inorganic Hybrids
;
_journal_issue                   5
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              1837
_journal_paper_doi               10.1021/cg050100m
_journal_volume                  5
_journal_year                    2005
_chemical_formula_moiety         'Mo8 O26, 2(C6 H10 N2), 6(H2 O)'
_chemical_formula_sum            'C12 H32 Mo8 N4 O32'
_chemical_formula_weight         1511.94
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 99.415(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   8.3431(9)
_cell_length_b                   21.468(3)
_cell_length_c                   10.2766(12)
_cell_measurement_reflns_used    3326
_cell_measurement_temperature    273(2)
_cell_measurement_theta_max      28.28
_cell_measurement_theta_min      2.22
_cell_volume                     1815.8(4)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      273(2)
_diffrn_measured_fraction_theta_full 0.956
_diffrn_measured_fraction_theta_max 0.956
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0283
_diffrn_reflns_av_sigmaI/netI    0.0335
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            9491
_diffrn_reflns_theta_full        25.49
_diffrn_reflns_theta_max         25.49
_diffrn_reflns_theta_min         1.90
_exptl_absorpt_coefficient_mu    2.784
_exptl_absorpt_correction_T_max  0.808
_exptl_absorpt_correction_T_min  0.530
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Bruker, 2000)'
_exptl_crystal_colour            'pale yellow'
_exptl_crystal_density_diffrn    2.765
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             1448
_exptl_crystal_size_max          0.342
_exptl_crystal_size_mid          0.192
_exptl_crystal_size_min          0.078
_refine_diff_density_max         0.556
_refine_diff_density_min         -0.528
_refine_diff_density_rms         0.115
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.086
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     261
_refine_ls_number_reflns         3221
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.086
_refine_ls_R_factor_all          0.0390
_refine_ls_R_factor_gt           0.0313
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0245P)²+3.1471P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0657
_refine_ls_wR_factor_ref         0.0686
_reflns_number_gt                2786
_reflns_number_total             3367
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg050100msi20050318_012622.cif
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_H-M      P2(1)/n
_cod_database_code               4505139
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mo1 Mo 0.52831(5) 0.123050(19) 0.76267(4) 0.02102(12) Uani 1 1 d .
Mo2 Mo 0.64208(5) -0.118815(18) 0.97289(4) 0.02158(12) Uani 1 1 d .
Mo3 Mo 0.45741(5) -0.025956(19) 0.72113(4) 0.02139(12) Uani 1 1 d .
Mo4 Mo 0.70648(5) 0.026968(18) 1.01513(4) 0.01901(12) Uani 1 1 d .
O1 O 0.6518(4) 0.17473(16) 0.7023(3) 0.0337(9) Uani 1 1 d .
O2 O 0.3407(4) 0.13508(15) 0.6727(3) 0.0287(8) Uani 1 1 d .
O3 O 0.4956(4) 0.16195(14) 0.9244(3) 0.0227(7) Uani 1 1 d .
O4 O 0.7456(4) 0.08660(15) 0.9095(3) 0.0230(8) Uani 1 1 d .
O5 O 0.5775(4) 0.04632(14) 0.6840(3) 0.0220(7) Uani 1 1 d .
O6 O 0.4386(4) 0.04145(14) 0.8988(3) 0.0199(7) Uani 1 1 d .
O7 O 0.8877(4) 0.01031(16) 1.1083(3) 0.0284(8) Uani 1 1 d .
O8 O 0.6877(4) -0.04042(14) 0.8856(3) 0.0200(7) Uani 1 1 d .
O9 O 0.8279(4) -0.12897(16) 1.0650(3) 0.0320(9) Uani 1 1 d .
O10 O 0.6337(5) -0.17083(16) 0.8471(3) 0.0338(9) Uani 1 1 d .
O11 O 0.3939(4) -0.07797(14) 0.8632(3) 0.0188(7) Uani 1 1 d .
O12 O 0.5338(5) -0.08004(16) 0.6284(3) 0.0339(9) Uani 1 1 d .
O13 O 0.2692(4) -0.00858(17) 0.6383(3) 0.0321(9) Uani 1 1 d .
C1 C 0.8040(6) 0.2038(2) 0.1991(5) 0.0260(12) Uani 1 1 d .
C2 C 0.9411(7) 0.1742(2) 0.1727(5) 0.0355(14) Uani 1 1 d .
H2 H 0.9751 0.1796 0.0916 0.043 Uiso 1 1 calc R
C3 C 1.0277(7) 0.1364(2) 0.2679(5) 0.0325(13) Uani 1 1 d .
H3 H 1.1200 0.1156 0.2511 0.039 Uiso 1 1 calc R
C4 C 0.9767(6) 0.1297(2) 0.3872(5) 0.0250(11) Uani 1 1 d .
C5 C 0.8404(6) 0.1597(2) 0.4143(5) 0.0299(12) Uani 1 1 d .
H5 H 0.8063 0.1540 0.4952 0.036 Uiso 1 1 calc R
C6 C 0.7546(7) 0.1984(2) 0.3202(5) 0.0318(13) Uani 1 1 d .
H6 H 0.6648 0.2204 0.3384 0.038 Uiso 1 1 calc R
N1 N 0.7034(5) 0.23980(18) 0.0955(4) 0.0289(10) Uani 1 1 d .
H1A H 0.7670 0.2606 0.0491 0.043 Uiso 1 1 calc R
H1B H 0.6424 0.2666 0.1320 0.043 Uiso 1 1 calc R
H1C H 0.6395 0.2141 0.0423 0.043 Uiso 1 1 calc R
N2 N 1.0658(5) 0.08679(19) 0.4849(4) 0.0288(10) Uani 1 1 d .
H2A H 1.0988 0.0539 0.4437 0.043 Uiso 1 1 calc R
H2B H 1.0009 0.0743 0.5404 0.043 Uiso 1 1 calc R
H2C H 1.1517 0.1063 0.5297 0.043 Uiso 1 1 calc R
O1W O 0.9981(6) 0.1811(2) 0.7117(4) 0.0480(11) Uani 1 1 d .
O2W O 0.6186(6) 0.7924(2) 0.5754(4) 0.0564(13) Uani 1 1 d .
O3W O 0.8973(5) 0.02281(16) 0.6587(4) 0.0324(9) Uani 1 1 d .
H1W H 1.0637 0.1611 0.7668 0.05(2) Uiso 1 1 d R
H6W H 0.9421 0.0232 0.7255 0.05(2) Uiso 1 1 d R
H2W H 0.9019 0.1799 0.6909 0.08(3) Uiso 1 1 d R
H5W H 0.8085 0.0297 0.6572 0.05(2) Uiso 1 1 d R
H4W H 0.6362 0.8162 0.6333 0.10(3) Uiso 1 1 d R
H3W H 0.5855 0.7756 0.6371 0.26(8) Uiso 1 1 d R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Mo1 O2 105.14(17) . .
O1 Mo1 O5 102.91(15) . .
O2 Mo1 O5 98.24(15) . .
O1 Mo1 O3 102.29(15) . .
O2 Mo1 O3 98.98(15) . .
O5 Mo1 O3 144.41(13) . .
O1 Mo1 O4 90.10(15) . .
O2 Mo1 O4 164.75(14) . .
O5 Mo1 O4 77.46(13) . .
O3 Mo1 O4 77.77(13) . .
O1 Mo1 O6 160.30(15) . .
O2 Mo1 O6 94.55(14) . .
O5 Mo1 O6 74.34(11) . .
O3 Mo1 O6 73.43(11) . .
O4 Mo1 O6 70.21(11) . .
O9 Mo2 O10 105.09(18) . .
O9 Mo2 O3 101.88(15) . 3_657
O10 Mo2 O3 98.47(15) . 3_657
O9 Mo2 O8 97.88(15) . .
O10 Mo2 O8 101.61(14) . .
O3 Mo2 O8 146.97(13) 3_657 .
O9 Mo2 O6 95.73(15) . 3_657
O10 Mo2 O6 159.18(15) . 3_657
O3 Mo2 O6 76.98(12) 3_657 3_657
O8 Mo2 O6 74.92(11) . 3_657
O9 Mo2 O11 165.24(14) . .
O10 Mo2 O11 87.54(15) . .
O3 Mo2 O11 83.38(12) 3_657 .
O8 Mo2 O11 71.65(12) . .
O6 Mo2 O11 71.81(11) 3_657 .
O12 Mo3 O13 105.71(18) . .
O12 Mo3 O5 100.72(15) . .
O13 Mo3 O5 101.10(16) . .
O12 Mo3 O11 101.50(15) . .
O13 Mo3 O11 99.00(15) . .
O5 Mo3 O11 144.58(13) . .
O12 Mo3 O6 159.65(15) . .
O13 Mo3 O6 94.60(14) . .
O5 Mo3 O6 76.15(11) . .
O11 Mo3 O6 73.43(11) . .
O12 Mo3 O8 88.59(15) . .
O13 Mo3 O8 164.41(14) . .
O5 Mo3 O8 81.86(13) . .
O11 Mo3 O8 71.50(12) . .
O6 Mo3 O8 71.08(11) . .
O7 Mo4 O4 105.47(16) . .
O7 Mo4 O11 101.17(15) . 3_657
O4 Mo4 O11 97.52(14) . 3_657
O7 Mo4 O8 101.16(15) . .
O4 Mo4 O8 96.99(14) . .
O11 Mo4 O8 148.96(13) 3_657 .
O7 Mo4 O6 97.60(14) . 3_657
O4 Mo4 O6 156.93(14) . 3_657
O11 Mo4 O6 78.06(12) 3_657 3_657
O8 Mo4 O6 77.86(12) . 3_657
O7 Mo4 O6 173.31(14) . .
O4 Mo4 O6 81.21(13) . .
O11 Mo4 O6 77.42(12) 3_657 .
O8 Mo4 O6 77.89(12) . .
O6 Mo4 O6 75.72(12) 3_657 .
Mo1 O3 Mo2 116.66(16) . 3_657
Mo4 O4 Mo1 116.80(16) . .
Mo1 O5 Mo3 117.26(15) . .
Mo4 O6 Mo2 91.15(11) 3_657 3_657
Mo4 O6 Mo3 90.72(11) 3_657 .
Mo2 O6 Mo3 162.86(16) 3_657 .
Mo4 O6 Mo4 104.28(12) 3_657 .
Mo2 O6 Mo4 98.40(12) 3_657 .
Mo3 O6 Mo4 97.65(11) . .
Mo4 O6 Mo1 163.92(16) 3_657 .
Mo2 O6 Mo1 87.47(10) 3_657 .
Mo3 O6 Mo1 86.04(10) . .
Mo4 O6 Mo1 91.76(11) . .
Mo4 O8 Mo2 108.75(14) . .
Mo4 O8 Mo3 110.80(13) . .
Mo2 O8 Mo3 104.04(14) . .
Mo4 O11 Mo3 110.57(14) 3_657 .
Mo4 O11 Mo2 109.72(13) 3_657 .
Mo3 O11 Mo2 104.02(13) . .
C2 C1 C6 121.4(5) . .
C2 C1 N1 119.8(4) . .
C6 C1 N1 118.7(5) . .
C1 C2 C3 119.2(5) . .
C1 C2 H2 120.4 . .
C3 C2 H2 120.4 . .
C4 C3 C2 119.5(5) . .
C4 C3 H3 120.2 . .
C2 C3 H3 120.2 . .
C3 C4 C5 121.4(5) . .
C3 C4 N2 118.7(5) . .
C5 C4 N2 119.8(4) . .
C4 C5 C6 119.4(5) . .
C4 C5 H5 120.3 . .
C6 C5 H5 120.3 . .
C1 C6 C5 119.0(5) . .
C1 C6 H6 120.5 . .
C5 C6 H6 120.5 . .
C1 N1 H1A 109.5 . .
C1 N1 H1B 109.5 . .
H1A N1 H1B 109.5 . .
C1 N1 H1C 109.5 . .
H1A N1 H1C 109.5 . .
H1B N1 H1C 109.5 . .
C4 N2 H2A 109.5 . .
C4 N2 H2B 109.5 . .
H2A N2 H2B 109.5 . .
C4 N2 H2C 109.5 . .
H2A N2 H2C 109.5 . .
H2B N2 H2C 109.5 . .
H1W O1W H2W 133.1 . .
H4W O2W H3W 75.1 . .
H6W O3W H5W 111.7 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O1 1.699(3) .
Mo1 O2 1.703(4) .
Mo1 O5 1.909(3) .
Mo1 O3 1.919(3) .
Mo1 O4 2.298(3) .
Mo1 O6 2.435(3) .
Mo2 O9 1.694(4) .
Mo2 O10 1.701(3) .
Mo2 O3 1.920(3) 3_657
Mo2 O8 1.973(3) .
Mo2 O6 2.289(3) 3_657
Mo2 O11 2.359(3) .
Mo3 O12 1.691(3) .
Mo3 O13 1.701(4) .
Mo3 O5 1.919(3) .
Mo3 O11 1.978(3) .
Mo3 O6 2.355(3) .
Mo3 O8 2.363(3) .
Mo4 O7 1.690(3) .
Mo4 O4 1.743(3) .
Mo4 O11 1.951(3) 3_657
Mo4 O8 1.955(3) .
Mo4 O6 2.180(3) 3_657
Mo4 O6 2.377(3) .
O3 Mo2 1.920(3) 3_657
O6 Mo4 2.180(3) 3_657
O6 Mo2 2.289(3) 3_657
O11 Mo4 1.951(3) 3_657
C1 C2 1.373(7) .
C1 C6 1.379(7) .
C1 N1 1.464(6) .
C2 C3 1.382(7) .
C2 H2 0.9300 .
C3 C4 1.370(7) .
C3 H3 0.9300 .
C4 C5 1.375(7) .
C4 N2 1.471(6) .
C5 C6 1.382(7) .
C5 H5 0.9300 .
C6 H6 0.9300 .
N1 H1A 0.8900 .
N1 H1B 0.8900 .
N1 H1C 0.8900 .
N2 H2A 0.8900 .
N2 H2B 0.8900 .
N2 H2C 0.8900 .
O1W H1W 0.8378 .
O1W H2W 0.7968 .
O2W H4W 0.7784 .
O2W H3W 0.8158 .
O3W H6W 0.7261 .
O3W H5W 0.7528 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O1 Mo1 O3 Mo2 179.42(18) . 3_657
O2 Mo1 O3 Mo2 71.7(2) . 3_657
O5 Mo1 O3 Mo2 -46.4(3) . 3_657
O4 Mo1 O3 Mo2 -93.19(18) . 3_657
O6 Mo1 O3 Mo2 -20.46(16) . 3_657
O7 Mo4 O4 Mo1 179.51(16) . .
O11 Mo4 O4 Mo1 -76.65(17) 3_657 .
O8 Mo4 O4 Mo1 75.84(17) . .
O6 Mo4 O4 Mo1 0.5(4) 3_657 .
O6 Mo4 O4 Mo1 -0.70(14) . .
O1 Mo1 O4 Mo4 179.85(19) . .
O2 Mo1 O4 Mo4 -1.9(6) . .
O5 Mo1 O4 Mo4 -76.94(18) . .
O3 Mo1 O4 Mo4 77.29(18) . .
O6 Mo1 O4 Mo4 0.71(15) . .
O1 Mo1 O5 Mo3 -177.84(19) . .
O2 Mo1 O5 Mo3 -70.2(2) . .
O3 Mo1 O5 Mo3 48.1(3) . .
O4 Mo1 O5 Mo3 94.97(18) . .
O6 Mo1 O5 Mo3 22.30(16) . .
O12 Mo3 O5 Mo1 177.69(19) . .
O13 Mo3 O5 Mo1 69.2(2) . .
O11 Mo3 O5 Mo1 -54.3(3) . .
O6 Mo3 O5 Mo1 -22.90(17) . .
O8 Mo3 O5 Mo1 -95.31(18) . .
O12 Mo3 O6 Mo4 -96.5(4) . 3_657
O13 Mo3 O6 Mo4 79.69(15) . 3_657
O5 Mo3 O6 Mo4 -179.99(14) . 3_657
O11 Mo3 O6 Mo4 -18.34(12) . 3_657
O8 Mo3 O6 Mo4 -93.98(12) . 3_657
O12 Mo3 O6 Mo2 167.2(5) . 3_657
O13 Mo3 O6 Mo2 -16.6(5) . 3_657
O5 Mo3 O6 Mo2 83.8(5) . 3_657
O11 Mo3 O6 Mo2 -114.6(5) . 3_657
O8 Mo3 O6 Mo2 169.8(5) . 3_657
O12 Mo3 O6 Mo4 8.0(4) . .
O13 Mo3 O6 Mo4 -175.80(14) . .
O5 Mo3 O6 Mo4 -75.48(13) . .
O11 Mo3 O6 Mo4 86.17(13) . .
O8 Mo3 O6 Mo4 10.53(10) . .
O12 Mo3 O6 Mo1 99.2(4) . .
O13 Mo3 O6 Mo1 -84.55(14) . .
O5 Mo3 O6 Mo1 15.77(12) . .
O11 Mo3 O6 Mo1 177.42(14) . .
O8 Mo3 O6 Mo1 101.78(11) . .
O4 Mo4 O6 Mo4 179.53(15) . 3_657
O11 Mo4 O6 Mo4 -80.68(13) 3_657 3_657
O8 Mo4 O6 Mo4 80.37(13) . 3_657
O6 Mo4 O6 Mo4 0.0 3_657 3_657
O4 Mo4 O6 Mo2 -87.12(14) . 3_657
O11 Mo4 O6 Mo2 12.68(11) 3_657 3_657
O8 Mo4 O6 Mo2 173.73(14) . 3_657
O6 Mo4 O6 Mo2 93.36(13) 3_657 3_657
O4 Mo4 O6 Mo3 86.82(13) . .
O11 Mo4 O6 Mo3 -173.38(13) 3_657 .
O8 Mo4 O6 Mo3 -12.33(11) . .
O6 Mo4 O6 Mo3 -92.71(13) 3_657 .
O4 Mo4 O6 Mo1 0.59(12) . .
O11 Mo4 O6 Mo1 100.38(12) 3_657 .
O8 Mo4 O6 Mo1 -98.57(12) . .
O6 Mo4 O6 Mo1 -178.94(17) 3_657 .
O1 Mo1 O6 Mo4 -179.3(5) . 3_657
O2 Mo1 O6 Mo4 2.6(5) . 3_657
O5 Mo1 O6 Mo4 -94.7(5) . 3_657
O3 Mo1 O6 Mo4 100.6(5) . 3_657
O4 Mo1 O6 Mo4 -176.8(6) . 3_657
O1 Mo1 O6 Mo2 95.3(4) . 3_657
O2 Mo1 O6 Mo2 -82.82(13) . 3_657
O5 Mo1 O6 Mo2 179.88(14) . 3_657
O3 Mo1 O6 Mo2 15.20(12) . 3_657
O4 Mo1 O6 Mo2 97.86(12) . 3_657
O1 Mo1 O6 Mo3 -100.6(4) . .
O2 Mo1 O6 Mo3 81.30(13) . .
O5 Mo1 O6 Mo3 -15.99(12) . .
O3 Mo1 O6 Mo3 179.33(14) . .
O4 Mo1 O6 Mo3 -98.01(12) . .
O1 Mo1 O6 Mo4 -3.0(4) . .
O2 Mo1 O6 Mo4 178.85(13) . .
O5 Mo1 O6 Mo4 81.55(13) . .
O3 Mo1 O6 Mo4 -83.12(13) . .
O4 Mo1 O6 Mo4 -0.47(10) . .
O7 Mo4 O8 Mo2 72.52(18) . .
O4 Mo4 O8 Mo2 179.87(16) . .
O11 Mo4 O8 Mo2 -62.8(3) 3_657 .
O6 Mo4 O8 Mo2 -22.95(15) 3_657 .
O6 Mo4 O8 Mo2 -100.72(16) . .
O7 Mo4 O8 Mo3 -173.71(15) . .
O4 Mo4 O8 Mo3 -66.37(16) . .
O11 Mo4 O8 Mo3 51.0(3) 3_657 .
O6 Mo4 O8 Mo3 90.81(14) 3_657 .
O6 Mo4 O8 Mo3 13.05(12) . .
O9 Mo2 O8 Mo4 -71.76(18) . .
O10 Mo2 O8 Mo4 -179.02(17) . .
O3 Mo2 O8 Mo4 54.7(3) 3_657 .
O6 Mo2 O8 Mo4 22.09(14) 3_657 .
O11 Mo2 O8 Mo4 97.54(15) . .
O9 Mo2 O8 Mo3 170.12(15) . .
O10 Mo2 O8 Mo3 62.85(17) . .
O3 Mo2 O8 Mo3 -63.4(3) 3_657 .
O6 Mo2 O8 Mo3 -96.04(13) 3_657 .
O11 Mo2 O8 Mo3 -20.59(10) . .
O12 Mo3 O8 Mo4 165.49(17) . .
O13 Mo3 O8 Mo4 -37.7(6) . .
O5 Mo3 O8 Mo4 64.45(15) . .
O11 Mo3 O8 Mo4 -91.89(15) . .
O6 Mo3 O8 Mo4 -13.62(12) . .
O12 Mo3 O8 Mo2 -77.80(16) . .
O13 Mo3 O8 Mo2 79.0(5) . .
O5 Mo3 O8 Mo2 -178.84(14) . .
O11 Mo3 O8 Mo2 24.82(12) . .
O6 Mo3 O8 Mo2 103.09(14) . .
O12 Mo3 O11 Mo4 -178.27(17) . 3_657
O13 Mo3 O11 Mo4 -70.09(19) . 3_657
O5 Mo3 O11 Mo4 53.9(3) . 3_657
O6 Mo3 O11 Mo4 22.06(14) . 3_657
O8 Mo3 O11 Mo4 97.16(16) . 3_657
O12 Mo3 O11 Mo2 64.02(17) . .
O13 Mo3 O11 Mo2 172.19(15) . .
O5 Mo3 O11 Mo2 -63.8(2) . .
O6 Mo3 O11 Mo2 -95.65(13) . .
O8 Mo3 O11 Mo2 -20.55(10) . .
O9 Mo2 O11 Mo4 -47.3(6) . 3_657
O10 Mo2 O11 Mo4 163.44(17) . 3_657
O3 Mo2 O11 Mo4 64.62(15) 3_657 3_657
O8 Mo2 O11 Mo4 -93.47(15) . 3_657
O6 Mo2 O11 Mo4 -13.81(12) 3_657 3_657
O9 Mo2 O11 Mo3 71.0(5) . .
O10 Mo2 O11 Mo3 -78.26(16) . .
O3 Mo2 O11 Mo3 -177.08(15) 3_657 .
O8 Mo2 O11 Mo3 24.83(12) . .
O6 Mo2 O11 Mo3 104.49(14) 3_657 .
C6 C1 C2 C3 2.4(8) . .
N1 C1 C2 C3 -174.8(5) . .
C1 C2 C3 C4 -0.8(8) . .
C2 C3 C4 C5 0.2(8) . .
C2 C3 C4 N2 177.0(5) . .
C3 C4 C5 C6 -1.2(8) . .
N2 C4 C5 C6 -178.0(5) . .
C2 C1 C6 C5 -3.4(8) . .
N1 C1 C6 C5 173.9(5) . .
C4 C5 C6 C1 2.7(8) . .
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 PubChem 139145732
